Dimensional reduction upon calcium incorporation in Cs0.3(Ca0.3Ln0.7)PS4 and Cs0.5(Ca0.5Ln0.5)PS4
Klepov, Vladislav V.; Kocevski, Vancho; Besmann, Theodore M.; zur Loye, Hans-Conrad; CrystEngComm 23 (2021) 831–840; doi:10.1039/D0CE01524E

data_7241722
_publ_section_title
;
 Dimensional reduction upon calcium incorporation in Cs0.3(Ca0.3Ln0.7)PS4
 and Cs0.5(Ca0.5Ln0.5)PS4
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              831
_journal_page_last               840
_journal_paper_doi               10.1039/D0CE01524E
_journal_volume                  23
_journal_year                    2021
_chemical_formula_sum            'Ca0.3 Cs0.3 P S4 Tb0.7'
_chemical_formula_weight         322.35
_space_group_crystal_system      trigonal
_space_group_IT_number           166
_space_group_name_Hall           '-R 3 2"'
_space_group_name_H-M_alt        'R -3 m :H'
_audit_creation_method           SHELXL-2018/1
_audit_update_record
;
2020-10-14 deposited with the CCDC.	2020-12-01 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   16.3448(4)
_cell_length_b                   16.3448(4)
_cell_length_c                   13.3425(3)
_cell_measurement_reflns_used    9404
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      33.11
_cell_measurement_theta_min      3.26
_cell_volume                     3086.93(13)
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0243
_diffrn_reflns_av_unetI/netI     0.0069
_diffrn_reflns_Laue_measured_fraction_full 0.987
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            30233
_diffrn_reflns_point_group_measured_fraction_full 0.987
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.499
_diffrn_reflns_theta_min         3.258
_exptl_absorpt_coefficient_mu    10.379
_exptl_absorpt_correction_T_max  0.2694
_exptl_absorpt_correction_T_min  0.2210
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 Reference: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.121
_exptl_crystal_description       block
_exptl_crystal_F_000             2646
_exptl_crystal_size_max          0.030
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.020
_refine_diff_density_max         3.038
_refine_diff_density_min         -4.245
_refine_diff_density_rms         0.187
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.126
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_reflns         875
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.126
_refine_ls_R_factor_all          0.0298
_refine_ls_R_factor_gt           0.0298
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0492P)^2^+54.2359P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0878
_refine_ls_wR_factor_ref         0.0878
_reflns_Friedel_coverage         0.000
_reflns_number_gt                874
_reflns_number_total             875
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0ce01524e2.cif
_cod_data_source_block           Tb07
_cod_depositor_comments
'Adding full bibliography for 7241712--7241724.cif.'
_cod_original_cell_volume        3086.93(17)
_cod_original_formula_sum        'Ca0.30 Cs0.30 P S4 Tb0.70'
_cod_database_code               7241722
_shelx_shelxl_version_number     2018/1
_shelx_estimated_absorpt_t_min   0.746
_shelx_estimated_absorpt_t_max   0.819
_shelx_res_checksum              9953